Crystal growth, structural characterization, cation‒cation interaction classification, and optical properties of uranium(vi) containing oxychlorides, A4U5O16Cl2(A = K, Rb), Cs5U7O22Cl3, and AUO3Cl (A = Rb, Cs)
Read, Cory Michael; Yeon, Jeongho; Smith, Mark D.; zur Loye, Hans-Conrad; CrystEngComm 16 (2014) 7259–; doi:10.1039/C4CE00281D

data_7217418
_publ_section_title
;
 Crystal growth, structural characterization, cation--cation interaction
 classification, and optical properties of uranium(vi) containing
 oxychlorides, A4U5O16Cl2(A = K, Rb), Cs5U7O22Cl3, and AUO3Cl (A = Rb, Cs)
;
_journal_issue                   31
_journal_name_full               CrystEngComm
_journal_page_first              7259
_journal_paper_doi               10.1039/C4CE00281D
_journal_volume                  16
_journal_year                    2014
_chemical_formula_moiety         'Cl3 Cs5 O22 U7'
_chemical_formula_sum            'Cl3 Cs5 O22 U7'
_chemical_formula_weight         2789.11
_chemical_name_systematic
;
 ? 
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             2013-05-08
_audit_creation_method
;
  Olex2 1.2
  (compiled Apr 23 2013 17:59:47, GUI svn.r4466)
;
_cell_angle_alpha                90.00
_cell_angle_beta                 102.9850(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   10.6214(5)
_cell_length_b                   18.1071(8)
_cell_length_c                   16.0857(7)
_cell_measurement_reflns_used    4341
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      31.16
_cell_measurement_theta_min      2.60
_cell_volume                     3014.5(2)
_computing_cell_refinement       'SAINT v6.45A (Bruker, 2003)'
_computing_data_reduction        'SAINT v6.45A (Bruker, 2003)'
_computing_molecular_graphics
;
O. V. Dolomanov, L. J. Bourhis, R. J. Gildea, J. A. K. Howard and H. Puschmann,
OLEX2: a complete structure solution, refinement and analysis program.
J. Appl. Cryst. (2009). 42, 339-341.
;
_computing_publication_material
;
O. V. Dolomanov, L. J. Bourhis, R. J. Gildea, J. A. K. Howard and H. Puschmann,
OLEX2: a complete structure solution, refinement and analysis program.
J. Appl. Cryst. (2009). 42, 339-341.
;
_computing_structure_refinement
;
SHELXL, G.M. Sheldrick, Acta Cryst.
(2008). A64, 112-122
;
_computing_structure_solution
;
SHELXS, G.M. Sheldrick, Acta Cryst.
(2008). A64, 112-122
;
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1058
_diffrn_reflns_av_unetI/netI     0.0563
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            84222
_diffrn_reflns_theta_full        31.50
_diffrn_reflns_theta_max         31.50
_diffrn_reflns_theta_min         1.72
_diffrn_source                   'fine-focus sealed tube'
_diffrn_source_current           35.0
_diffrn_source_power             1.575
_diffrn_source_target            Mo
_diffrn_source_voltage           45.0
_exptl_absorpt_coefficient_mu    43.755
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.263689
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS v.2.10 (Bruker,2003) was used for absorption correction.
R(int) was 0.2003 before and 0.0623 after correction.
The Ratio of minimum to maximum transmission is 0.2637.
The \l/2 correction factor is 0.0015.
;
_exptl_crystal_colour            Orange
_exptl_crystal_colour_primary    orange
_exptl_crystal_density_diffrn    6.145
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             4584
_exptl_crystal_size_max          0.06
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.03
_refine_diff_density_max         2.204
_refine_diff_density_min         -2.001
_refine_diff_density_rms         0.458
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.032
_refine_ls_matrix_type           full
_refine_ls_number_parameters     337
_refine_ls_number_reflns         10051
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.032
_refine_ls_R_factor_all          0.0628
_refine_ls_R_factor_gt           0.0409
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0259P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0734
_refine_ls_wR_factor_ref         0.0808
_reflns_number_gt                7724
_reflns_number_total             10051
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c4ce00281d2.cif
_cod_data_source_block           Cs5U7O22Cl3
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_colour_primary' value 'Orange' changed to 'orange'
according to
/usr/data/users/saulius/crontab/automatic-downloads/current/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 
;
_cod_database_code               7217418
_olex2_refinement_description
;
;